Disclosure to Promote the Right To Information Whereas the Parliament of India has set out to provide a practical regime of right to information for citizens to secure access to information under the control of public authorities, in order to promote transparency and accountability in the working of every public authority, and whereas the attached publication of the Bureau of Indian Standards is of particular interest to the public, particularly disadvantaged communities and those engaged in the pursuit of education and knowledge, the attached public safety standard is made available to promote the timely dissemination of this information in an accurate manner to the public. “जान1 का अ+धकार, जी1 का अ+धकार”
“प0रा1 को छोड न' 5 तरफ”
“The Right to Information, The Right to Live”
“Step Out From the Old to the New”
Mazdoor Kisan Shakti Sangathan
IS 2386-4 (1963): Methods of test for aggregates for concrete, Part 4: Mechanical properties [CED 2: Cement and Concrete]
“!ान $ एक न' भारत का +नम-ण” Satyanarayan Gangaram Pitroda
“Invent a New India Using Knowledge”
“!ान एक ऐसा खजाना > जो कभी च0राया नहB जा सकता ह” है” ह Bhartṛhari—Nītiśatakam
“Knowledge is such a treasure which cannot be stolen”
IS :2366 ( Part IV ) - 1963 Reaffirmed 2002 1990 ) (( Reaffirmed
Indian Standard METHODS OF TEST FOR AGGREGATES FOR CONCRETE PART IV MECHANICAL
Tenth Reprint MARCH 1997 ( Incorporating Amendment No. 1 )
STANDARDS SHAH ZAFAR MARC;
IS : 2386 ( Part IV ) - 1963
Indian Standard METHODS OF TEST FOR AGGREGATES FOR CONCRETE PART IV MECHANICAL
and Concrete Sectional Committee, BDC 2
SHRI K. K. NAM~IAR
Members SHRI K. V. THADANEY (Allcmalc
Shri K. K. Nambiar) SIIIU K. F. ANTIA
M. N. Dastur
YHRI P. S. BHATNAGAR
I. C. DOS M. PAIS CUDDOU
& Power) SHIU Y. K. MURTHV (ALcmafc) Snru N. D. DA~~ARY
SHRI N. G. DEWAN SUPEIUNTEND~N~Ewx-aen,
Central ZND Cmci%
>R R. R. HATTIAN~ADI
Stiat V. N. PAI (Altcrwfr) SHRI P. c.
(B & S)
of India, &
STANDARDS (B & S) (ANumcllc)
SHN S. B. JOSHI
S. B. Joshi
SHU M. M. La
SHU B. N. MAJU~DAR
SHP.~ P. L. DAS (Alfnnolc) Paw Smu
S. R. Manta
N. H. MOHILB
SHR~ S. N. MUKERJI SHRI N. C. %a~
ERACH A. NADIRSHAH
Smu C. B. PATEL
oi Engineers Buildings
& Rehabilitatl;on) Smu Rasr~o~n PROP
G. S. R~u.&sw#.rn~
SHR~ K. SIVA PRASAD (A~trmolc) Gammon
SHRI T. N. S. R.w
SHRI S. R. PINHEIRO (Altrrnof~)
(Continued on page 2)
9 BAHADUR SHAH ZAFAR NEW DELHI 110@02
IS : 2386 (Part IV) - 1963
& Power) Bnro
G. S. Sntora Smtr
R. S. MEHANDRU SU~~ARAJU
SHRI J. M. TREHAN
SHRI N. H. K~swn~r Director
(Alfern&) Dircc tar,
DR. H. C. V~SVESV~RAYA, Deputy
Subcommittee, S. B. Josbi
STANDARDS (B & S)
I. C. DOS M. PAIS CVDOOU
Research, Designs Railways)
SHRI N. H. BHAGWANANI
& Power) Stint
Y. K. MURTHY
SHRI P. L. Das
Economic SHRI B. N. MAJUM~J~R
(Alfcnzolc) Engineering Ml~.zr&t~r
Research Pub!ic Buildings
Laboratory, Hyderabad WS_$” ‘.?=” I,mlr*mnn+ . . . . . .,... Organization
& Rehabilitatiotl) SHRI B. S. SIUVAMURTHY
SHIU C. L. Hanoa
& Power) SHRI P. C. Ha2n.a
K. K. NAMBIAR
SHRI C. L. N. IYP.NOER (A~fcmalc) DR. M. L. PURI PROF. G. S. Ramnsw~mv SHRI K. Stva
SHRI T. N. S. RAO <u-r 9 .x2. . .P,uul;..,rr .~ .._. “. . . . .._...I
I....“.,.“.“, SUPERINTENDING ENGINEER, ZND C~RCLB SHRI 0.
SIIR~ J. M. TREHAN
SHRI R. P. SIKKA (Altertrale) SHIU H. T. YAN
IS : 2386 (
IV ) - 1963
Indian Standard METHODS OF TEST FOR AGGREGATES FOR CONCRETE PART IV MECHANICAL
0.1 This Indian Standard (Part IV) was adopted by the Indian Standards Institution on 24 September 1963, after the draft finalized by the Cement and Concrete Sectional Committee had been approved by the Building Division Council. 0.2 One of the major contributing factors to the quality of concrete is the The test methods given in this standard quality of aggregates used therein. In a given are intended to assist in assessing the quality of aggregates. situation, for a particular aggregate, it may not be necessary to assess all the qualities and therefore it is necessary to determine beforehand the purpose for which a concrete is being used and the qualities of the aggregate which Accordingly, the relevant test methods may be require to be assessed. chosen from amongst the various tests covered in this standard. For the convenience of the users, the test methods are grouped into the following eight parts of Indian Standard Methods of Test for Aggregates for Concrete (IS : 2386-1963) : Part
Size and Shape
of Fine Aggregate
0.3 The Sectional Committee responsible for the preparation of this standard has taken into consideration the views of concrete specialists, testing authorities, consumers and technologists and has related the standard to the Further, the need for international practices followed in this country. co-ordination among standards prevailing in different countries of the world These considerations led the Sectional Committee has also been recognized. 3
I§ : 2386 (Part IV) - 1963 to derive assistance from the puhlished following organizations: British Standards American
Society for Testing
0.4 Wherever a reference to any Indian Standard it shall be taken as a reference to its latest version.
appears in these methods,
0.5 For the purpose of deciding whether a particular requirement of this standard is complied with, the final value, observed or calculated, expressing the result of a test or analysis, shall be rounded off in accordance with IS : Z-1960 Rules for Rounding Off Numerical Values (Revised). The number of significant places retained in the rounded off value should be the same as that of the specified value in this standard. 0.6 This standard is intended chiefly to cover the technical provisions relating to testing of aggregates for concrete, and it does not include all the necessary provisions of a contract.
1. SCOPE 1.1 This
covers the following
tests for aggregates
concrete : a) Determination
of the 10 percent
of the Polished Stone Value,
2.1 Object aggregate
Vaiue, Value, and
This method of test covers the procedure crushing value of coarse aggregate.
‘aggregate crushing value’ gives a relative measure of the resistance NOTE 1 -The of an aggregate to crushing under a gradually applied compressive load. With aggregate of ‘aggregate crushing value’ 30 or higher, the result may be anomalous, and in such cases the ‘ten percent fines value’ should be determined instead. NOTE 2 - The standard aggregate crushing test shall be made on aggre ate passing a 12.5-mm IS Sieve and retained on a IO-mm IS Sieve. If required, or if tRe standard size is not available, other sizes up to 25 mm may be tested but owing to the noIlchomogeneity of aggregates the results will not be comparable with those obtained in the standard (seeNote 1 under 2.6). Smaller sizes may also be tested (seeNote 2 under 2.6).
IS : 2386 (Part IV) â€˜- 1963 2.2 Apparatus following : a)
for the standard
test shall consist of the
15-cm diameter open-ended steel cylinder, with plunger and base-plate, of the general form and dimensions shown in Fig. 1. The surfaces in contact with the aggregate shall be machined and case-hardened or otherwise treated so as to have a diamond (VI-l) pyramid hardness number of not less than 650 VII. A
b) A straight metal tamping rod of circular cross-section diameter and 45 to 60 cm long, rounded at one end. c) A balance of capacity
3 kg, readable and accurate
d) IS Sieves of sizes 12.5,lO
16 mm in
to one gram.
and 2.36 mm.
e) A compression testing machine capable of applying a load of 46 tonnes and which can be operated to give a uniform rate of loading so that the maximum load is reached in 10 minutes. The machine may be used with or without a spherical seating. f) For measuring the sample, cylindrical metal measure of sufficient rigidity to retain its form under rough usage and of the following internal dimensions: Diameter
1 l-5 cm
2.3 Preparation of Test Sample - The material for the standard test shall consist of aggregate passing a 12.5-mm IS Sieve and retained on a IO-mm IS Sieve, and shall be thoroughly separated on these sieves before testing. For other sizes, the material shall be separated on the appropriate sieves given in Table I. TABLE
DETAILS OF AGGREGATTZ CRUSHING TEST NON-STANDARDâ€™ SI2XS OF AGGREGATE +w.ws
2.3 and 2.4.2)
SUES (IS Smws)
SI7,E OF 1s
% 10 z5
20 12.5 6.3 4,75 3.35
15.0 15.0 or 7.5 15.0 15-o or 7.5
f:E z 1.70 mm 85Omiavzu 1.18 mm
15.0 or 7.5
NOTE - About 6.5 kg of natural aggregate b required to provide the two testsamples for the 15-cm cylinder, or about 1 kg for the 7.5~cm cylinder.
L8 I 2386 (Part IV) - 1963
Cylinder Internal diameter Height Wall thickness Plunger Diameter of piston Diameterof stem Height Depth of piston Diameter of hole (nominal)
Base-Platr Thickness (nominal) Side length of square
1522FO.5 130 to 140 C 16
77.zyO.5 70 to 80 C8
150&0.5 100 to 150 100 to 115 < 2.5 20
75.0 jyo.5 50 to 75 65 to 75
6.3 200 to 230
PRINCIPALDIMENSIONS OF APPARATUSFOR AWREGATE Cnmmca
If dried 2.3.1 The aggregate shall be tested in a surface-dry condition. by heating, the period of drying shall not exceed four hours, the temperature shall be 100 to 110Â°C and the aggregate shall be cooled to room temperature before testing. 2.3.2 The quantity of aggregate shall be such that the depth of material in the cylinder, after tamping as described in 2.3.3, shall be 10 cm. 2.3.3 The appropriate quantity may be found conveniently by filling the cylindrical measure in three layers of approximately equal depth, each layer being tamped 25 times with the rounded end of the tamping rod and finally levelled off, using the tamping rod as a straight-edge. 2.3.4 The weight of material comprising the test sample shall be determined (Weight A) and the same weight of sample shall be taken for the repeat test. 2.4 Test Procedure - The cylinder of the test apparatus shall be put in position on the base-plate and the test sample added in thirds, each third being subjected to 25 strokes from the tamping rod. The surface of the aggregate shall be carefully levelled and the plunger inserted so that it rests horizontally on this surface, care being taken to ensure that the plunger does not jam in the cylinder. 2.4.1 The apparatus, with the test sample and plunger in position, shall then be placed between the platens of the testing machine and loaded at as uniform a rate as possible so that the total load is reached in 10 minutes. The total load shall be 40 tonnes. 2.4.2 The load shall be released and the whole of the material removed from the cylinder and sieved on a 2.36-mm IS Sieve for the standard test, The fraction passing the sieve or the appropriate sieve given in Table I. shall be weighed (Weight B) . In all of these operations, Two tests shall be made.
care shall be taken
to avoid loss of the fines.
2.5 Calculation-The ratio of the weight of fines formed to the total s&nijIe weight in each test shall be expressed as a percentage, the result being recorded to the first decimal place: Aggregate
crushing value =
B = weight of fraction passing the appropriate A = weight of surface-dry 2.6 Reporting
of Results -
sample. The mean of the two results shall be reported 7
$S : 2386 (Part IV) - 1963 70the nearest whole number as the ‘aggregate crushing value’ of the size ob material tested, which shall be stated. NOTE 1 - A gregate larger than 12.5 mm - In general, the larger sizes of aggregate 3 er aggregate crushing value, but the relationship between the values will give a hlg Particular care obtained with different sizes will vary from one aggregate to another. shall be taken with larger sizes of aggregate to ensure that the plunger does not jam However, for such aggregate, a 7.5-cm diameter cylinder may be used, in the cylinder. and this has been found to give slightly higher results than the standard cylinder, so tbat the errors are compensating. NOTE 2 - Aggregafc smaller than 10 mm - In general, the smaller sizes of aggregate will give a lower aggregate crushing value, but the relationship between the values obtained with different sizes will vary from one aggregate to another.
For testing aggregate smaller than 10 mm:
The form and dimensions of the 7.5-cm cylinder shall be as shown in Fig. 1 and the surfaces shall be as for the standard cylinder.
The tamping rod shall be 8 mm in diameter and 30 cm long, rounded at one end.
The balance shall be of capacity to 02 g.
500 g, readable
4 The e) The
IS Sieves shall be as given in Table I.
f 1 The g) The
metal measure shall be 6 cm in diameter and 9 cm in height.
compression testing machine shall be capable of applying a load of 10 tonnes uniformly in 10 minutes.
depth of material in the 7.5-cm cylinder shall be 5 cm after tamping.
The total load applied in 10 minutes shall be 10 tonnes.
Otherwise, the provisions of the standard test, as set out in 2.2 to 2.6 shall apply. 3. DETERMINATION
OF TEN PERCENT
3.1 Object - This method of test covers the procedure for determining the ‘ten percent fines’ value of coarse aggregates. NOTE- The ‘ten percent fines’ value gives a measure of the resistance of an aggregate to crushing, that is, applicable to all aggregates.
3.2 Apparatus folloM&lg:
The apparatus for the standard test shall consist of the
8) A 15-cm diameter open-ended steel cylinder, with plunger and base-plate, of the general form and dimensions shown in Fig. 1. The surfaces in contact with the aggregate shall be machined and case-hardened or otherwise treated so as to have a diamond (VH) pyramid hardness number of not less than 650 WI. 8
IS : 2386 (Part IV) - 1963 b) A straight metal tamping rod of circular cross-section diameter and 45 to 60 cm long, rounded at one end. c) A balance ofcapacity
3 kg, readable
d) The IS Sieve-s of sizes 12.5,
16 mm in
to one gram.
and 2.36 mm.
e) A compression testing machine capable of applying a load of 50 tonnes and which can be operated to give a uniform rate of loading so that the maximum load in any test is reached in 10 minutes. This load may vary from 0.5 to 50 tonnes. f) For measuring the sample, a cylindrical metal measure of sufficient rigidity to retain its form under rough usage and of the following internal dimensions : Diameter
g) Means of measuring the reduction in the distance between the platens of the testing machine to the nearest one millimetre during the test (for example, a dial gauge). 3.3 Preparation of Test Sample - The material for the test shall consist of aggregate passing a 12*5-mm IS Sieve and retained on a IO-mm IS Sieve and shall be thoroughly separated on these sieves before testing. 3.3.1 The aggregate shall be tested in a surface-dry condition. If dried by heating, the period of drying shall not exceed four hours, the temperature shall be 100 to 110Â°C and the aggregate shall, be cooled to room temperature before testing. 3.3.2 The quantity of aggregate shall be such that the depth of material in the cylinder, after tamping as described in 18.104.22.168, shall be 10 cm. 22.214.171.124 The appropriate quantity may be found conveniently by filling the cylindrical measure in three layers of approximately equal depth, each layer being tamped 25 times with the tamping rod and finally levelled off, using the tamping rod as a straight-edge, care being taken in the case of weaker materials not to break the particles. 3.3.3 The weight of material comprising the test sample shall be determined (Weight A) and the same weight of sample shall be taken for the repeat test. NOTE- About 65 kg of natural aggregate is required to provide the two test samples. Less of light-weight aggregate is required.
3.4 Test Procedure-The cylinder of the test apparatus shall be put in position on the base-plate and the test sample added in thirds, each third being subjected to 25 strokes from the tamping rod, care being taken in the case oE weak materials not to break the particles. The surface of the aggregate shall be carefully levelled and the plunger inserted so that it 9
IS : 2386 (Part IV) - 1963 rests horizontally on this surface, care being taken to ensure that the plunger does not jam in the cylinder. 3.4.1 The apparatus, with the test sample and plunger in position, shall then be placed in the compression testing machine. The load shall be applied at a uniform rate so as to cause a total penetration of the plunger in 10 minutes of about: 15.0 mm for rounded or partially rounded aggregates (for example, uncrushed gravels), 20.0 mm for normal crushed aggregates, and 24.0 mm for honeycombed aggregates (for example, expanded shales and slags). These figures may be varied according to the extent of the rounding or honeycombing. 3.4.2 After reaching the required maximum penetration, the load shall be released and the whole’ of the material removed from the cylinder and sieved on a 2.36-mm IS Sieve. The fines passing the sieve shall be weighed, and this weight expressed as a percentage of the weight of the test sample. Normally, this percentage will fall within the range 7.5 to 12.5, but if it does not, a further test shall be made at a load adjusted as seems appropriate to bring the percentage fines within the range of 7.5 to 12.5. NOTE-
The formula given in 3.5 may be used for calculating the load required.
3.4.3 A repeat test shall be made fines within the range 7.3 t’) 12.5.
at the load that
gives a percentage
3.5 Calculations - The mean percentage fines from the two tests at this load shall be used in the following formula to calculate the load required to give 10 percent fines: 14xx Load required for 10 percent fines= YS4 where x = load in tonnes, and y = mean
fines from two tests at x tonnes load.
load required to produce 10 percent 3.6 Reporting of Results -The fines shall be reported to the nearest whole number for loads of 10 tonnes or more, the nearest O-5 tonne for loads of less than 10 tonnes. 4. DETERMINATION
4.1 Object -. This method of test covers the procedure the aggregate impact value of coarse aggregate.
VALUE for determining
NOTE-The ‘aggregate impact value’ gives a relative measure of the resistance of an aggregate to sudden shock or impact, which in some aggregates differs from Its resistance to a slow compressive load.
IS : 2386 (Part IV) - 1963 4.2 Apparatus - The apparatus shall consist of the following: a) An impact testing machine of the general form shown in Fig. 2 and complying with the following: 1) Total weight not more than 60 kg nor less than 45 kg. 2) The machine shall have a metal base weighing between 22 and 30 kg with a plane lower surface of not less than 30 cm diameter, and shall be supported on a level and plane concrete or stone block or floor at least 45 cm thick. The machine shall be prevented from rocking either by fixing it to the block or floor or by supporting it on a level and plane metal plate cast into the surface of the block or floor. 3) A cylindrical steel cup of internal dimensions: Diameter 102 mm 50 mm Depth and not less than 6.3 mm thick with its inner surface casehardened, that can be rigidly fastened at the centre of the base and easily removed for emptying. 4) A metal tup or hammer weighing 13.5 to 14.0 kg, the lower end of which shall be cylindrical in shape, 100.0 mm in diameter and 5 cm long, with a 2-mm chamfer at the lower edge, and case-hardened. The hammer shall slide freely between vertical guides so arranged that the lower (cylindrical) part of the hammer is above and concentric with the cup. 5) Means for raising the hammer and allowing it to fall freely between the vertical guides from a height of 38OA5.0 mm on to the test sample in the cup, and means for adjusting the height of fall within 5 mm. 6) Means for supporting the hammer whilst fastening or removing the. cup. NOTE
Some means for automatically recording the number of blows is desirable.
IS Sieves of sizes 12.5,
10 and 2.36 mm.
c) Measure - A cylindrical metal measure, tared to the nearest gram, of sufficient rigidity to retain its form under rough usage, and of the following internal dimensions : Diameter 75 mm Depth 50 mm d) Tamping Rod-A straight metal tamping rod of circular cross-section 10 mm in diameter and 230 mm long, rounded at one end. e) Balance - A balance accurate to 0.1 g. f)
not less than 500 g, readable
Oven - A well-ventilated oven, thermostatically maintain a temperature of 100 to 110Â°C.
Is : 2386 (Part IV) - 1963 LOCKING PIN FOR MECHANISM
ADJUSTABLE STOP FOR RELEASE LIFTING HANDLE
RACHET COUNTER (TO COUNT NUMBER OF BLOWS)
CASE-HARDENED SURFACE TUP
CYLINDRICAL STEEL CUP INNER SURFACES CASE-HARDENED
All dimensions in millimetres. FIG. 2
AGGREGATE IMPACT TEST MACHINE
of the Test Sample
4.3.1 The test sample shall consist of aggregate the whole of which passes a 12.5-mm IS Sieve and is retained on a IO-mm IS Sieve. The aggregate comprising the test sample shall be dried in an oven for a period of four hours at a temperature of 100 to 110Â°C and cooled. 4.3.2 The measure shall be filled about one-third full with the aggregate and tamped with 25 strokes of the rounded end of the tamping rod. 12
IS : 2366 (Part IV) - 1963 further Gmilar quantity of aggregate shall be added and a further tamping of 25 strokes given. The measure shall finally be fined to overtlowmg, tamped 25 times and the surplus aggregate struck off, using the tamping The net weight of aggregate in the measure shall rod as a straight-edge. be determined to the nearest gram (Weight A) and this weight of aggregate shall be used for the duplicate test on the same material. 4.4
4.4.1 The impact machine shall rest without wedgirrg or packing the level plate, block or floor, so that it is rigid and the hammer columns are vertical.
4.4.2 The cup shall be fixed firmly in position on the base of the machine and the whole of the test sample placed in it and compacted by a single tamping of 25 strokes of the tamping rod. 4.4.3 The hammer the upper surface of on to the aggregate. such blows each being
shall be raised until its lower face is 380 mm above the aggregate in the cup, and allowed to fall freely The test sample shall be subjected to a total of 15 delivered at an interval of not less than one second.
4.4.4 The crushedâ€™ aggregate shall then be removed from the cup and the whole of it sieved on the 2*36-mm IS Sieve until no further significant The fraction passing the sieve shall be amount passes in one minute. The fraction retained on weighed to an accuracy of 0.1 g (Weight. e). the sieve shall also be weighed (Weight C) and, if the total weight (E+Y) is less than the initial weight (Weight A) by more than one gram, the result Two tests shall be made. shall be discarded and a fresh test made. 4.5 Calculations .-The ratio of the weight of fines formed to the total sample weight in each test shall he expressed as a percentage, the result being recorded to the first decimal place: Aggregate where R=\veight A =weight
4.6 Reporting of Results to the nearest whole number material. 5. DETERMINATION
impact value = + 2.36-mm
sample. The mean of the two results shall be reported as the aggregate impact value of the tested
5.1 Object -This test covers the following two methods the abrasion value of coarse aggregate: a) By the use of Deval machine (see 5.2), and b) By the use of Los Angeles machine (see 5.3). NOTE
VALUE of determining
\lâ€™hrrev-rr possible, method (b) should be preferred to m&od
IS : 2386 (Part IV) - 1963 5.2 Test for Abrasion Machine 5.2.1 Atparatus -
of Coarse apparatus
by the Use of iBeva1 of the
a) Deual machine - The Deval abrasion tes&ng machine shall consist of one or more hollow cast iron cylinders closed at one end and furnished with a tightly fitting iron cover at the other. The inside diameter of the cylinders shall be 20 cm and depth 34 cm. The cylinders shall be mounted on a shaft at an angle of 30 degrees with the axis of rotation of the shaft. b) Sieve--The
5.2.2 Abrasive Charge - The abrasive charge shall consist of 6 cast iron spheres or steel spheres approximately 48 mm in diameter, each weighing between 390 and 445 g. 126.96.36.199 An abrasive charge used with each test sample.
of 6 spheres weighing
10 g shall be
5.2.3 Grading - The coarse aggregate shall be separated by sieving in accordance with the sieve analysis specified in Part I of this standard into the various sizes required for grading the test sample according to one of the gradings specified in 5.2.4. The material thus separated into various sizes shall be washed and dried. 5.2.4 Test Sample - The test sample shall consist of dry coarse aggregate made up of percentages of the various sizes conforming to one of the gradings shown below. The grading used shall be that most nearly representing the coarse aggregate furnished for the work. Grading
Passing IS Sieve
Retained on IS Sieve
Percentage of Sam$e
20-mm 25-mm 40-mm 50-mm
12*5-mm 20-mm 25-mm 40-mm
9: 25 25
20-mm 25-mm 40-mm
12*5-mm 20-mm 25-mm
IS: 188.8.131.52 The weight of the test sample specific gravity and shall he as follows:
upon its average
Weight of Sample
Range in SpeciJic GraviQ Over 2.4 to 2.2 to Less than
g 5 500 5000
2.8 2.8 2.39 2.2
4 500 4 000
184.108.40.206 When the coarse aggregate furnished as much as 25 percent of material finer than 12.5 that either grading A, B or C would be used for the abrasion test shall be made, using grading D, if in the the particles less than 12.5 mm in size are not at to those particles 12.5 mm or over in size.
for the work mm hut is of abrasion test, opinion of the least equal in
contains such size a second engineer, hardness
220.127.116.11 Crushed gravel - In the case of crushed gravel, the test sample shall contain crushed fragments so as to be representative of the gravel furnished for the work and shall be prepared in accordance with 5.2.3, 18.104.22.168 and 22.214.171.124. NOTE-For
as a fragment
the purpose of this test, a crushed gravel fragment of gravel having at ,least one fractured face.
5.2.5 Procedure - The test sample and the abrasive charge shall be placed in the Deval abrasion testing machine and the machine rotated for 10 000 revolutions at a speed of 30 to 33 rev/min. At the completion of the test, the material shall be removed from the machine and sieved on a 1*70-mm IS Sieve. The material retained on the sieve shall be washed, dried, and accurately weighed to the nearest gram. 5.2.6
126.96.36.199 Percelttage of wear - The loss by abrasion shall be considered as the difference between the original weight of the test sample and the weight of the material retained on the 1.70-mm IS Sieve, expressed as percentage of the original weight of the test sample. 188.8.131.52 Crushed gravel - In the case of crushed gravel, the percentage by weight of crushed fragments shall be determined, and the permissible percentage or wear which shall be calculated as follows: w = ALf(lOO--A)Lâ€™ 100 where W = permissible
of wear, 15
Is : 2386 (Part IV) - 1963 A = percentage
L = maximum percentage of wear permitted by the specifications for gravel consisting entirely of uncrushed fragments, 100 --A
Lâ€™ = maximum for gravel 5.2.7
of crushed fragments,
percentage of wear permitted consisting entirely of crushed
Reporting of Results of wear,
of crushed fragments
5.3 Test for Abrasion Machine 5.3.1 Apparatus -
by the specifications fragments.
The report shall include the following:
in the test sample, and
of the test sample.
of Coarse Aggregates apparatus
by the Use of Los Angeles
shall consist of the following:
a) Los Angeles machine --- The Los Angeles abrasion testing machine, conforming in all its essential characteristics to the design shown in Fig. 3, shall be used. The machine shall consist of a hollow steel cylinder, closed at both ends, having an inside diameter of 700 mm and an inside length of 500 mm. The cylinder shall be mounted on stub shafts attached to the ends of&he cylinders but not entering it, and shall be mounted in such ,a manner that it may be rotated about its axis in a horizontal posit% .-â€˜&I opening in the cylinder shall be provided for the introduction of the test sample. The opening shall be closed dust-tight with a removable cover bolted in place. The cover shall be so designed as to maintain the cylindrical contour of the interior surface unless the shelf is so located that the charge will not fall on the cover, or come in contact with it during the test. A removable steel shelf, projecting radially 88 mm into the cylinder and extending its full length, shall be mounted along one element of the interior surface of the cylinder. The shelf shall be of such thickness and so mounted, by bolts or other approved means, as to be firm and rigid. The position of the shelf shall be such that the distance from the shelf to the opening, measured along the circumference of the cylinder in the direction of rotation, shall be not less than 1 250 mm. NOTE - The use of the shelf of wear-resistant steel, rectangular in cross-section and mounted independently of the cover, is preferred. However, a shelf consisting of a section of rolled angle, properly mounted on the inside of the cover plate, may be used, provided the direction of rotation is such that the charge will be caught.on the outside face of the angle. _
IS : 2386 (Part IV) - 1963
FILLER PLATE mm+ltlICKNESS
THICKNESS OF GASKET
PLATE STEEL SHELF 08x25~500 mm
PREFERRED DESIGN OF PLATE SHELF AND COVER
ALTERNATIVE DESIGN OF ANGLE SHELF CAST ENDS
STEEL OR NOT LESS
ROLLED STEEL THAN 12mm THI
NOTE 1 -
Shaft bearing will be mounted on concrete piers or other rigid supports.
NOTE 2 -Suggested
horse power for motor is not less than one. All dimensions in millimetres.
The I-70-mm IS Sieve.
5.3.2 Abrasive Charge-The abrasive charge shall consist of cast iron spheres or steel spheres approximately 48 mm in. diameter and each weighi% between 390 and 445 g. 17
IS : !Z3& (Part IV) - 1963 184.108.40.206 The abrasive charge, depending upon the grading sample as described in 5.3.3 shall be as follows : Grading
,Vumber of Spheres
of the tti
Weight of Charge g
A B C D
12 11 8
12 12 12
5 000&25 3 330&20
5 000&25 5 OOOf25
5.3.3 Test Sample - The test sample shall consist of clean aggregate which has been dried in an oven at 105 to 110Â°C to substantially constant weight and shall conform to one of the gradings shown in Table II. The grading or gradings used shall be those most nearly representing the aggregate furnished for the work. NOTE - It is recognized that different specification limits may be required for gradings E, F and G than for A, B, C and D. It is urged that investigations be conducted to determine the relationship, if any, which exists between results for these coarse gradings using the 10 000 g samples and the finer ones using the 5 000 g samples.
(Clause 5.3.3) %3VE SIZE (SQCARE HOLE) ____-h--___7
Passing mm 80 63 50 40 25 20 12.5
Retained mm 63 .iO 40 25 20 12.5 10
10 6.3 4.75
6.3 .4.75 2.36
1250 1250 1 250 1 250 *Tolerance
WEIGHT IN g OF TEST SAMPLE FOR GRADE ~-----.._.___ c: E F II
2500 2 500 -
2 500 2 500 -
of &2 percent permitted.
2 5002 2 500* 5 OOOf 5 ooo* 5 ooo* -
5 000â€™ 5000* -
IS : 2366 (Part IV) - 1963 5.3.4 Procedur. 220.127.116.11 The test sample and the abrasive charge shall be placed in the Los Angeles abrasion testing machine and the machine rotated at a speed of 20 to 33 rev/min. For gradings A, B, C and D, the machine shall be rotated for 500 revolutions; for gradings E, F and G, it shall be rotated for 1 000 revolutions. The machine shall be so driven and so counter-balanced as to maintain a substantially uniform peripheral speed. If an angle is used as the shelf, the machine shall be rotated in such a direction that the charge is caught on the outside surface of the angle. At the .completion of the test, the material shall be discharged from the machine and a preliminary separation of the sample made on a sieve coarser than the l-70-mm IS Sieve. The finer portion shall then be sieved on a 1.70-mm IS Sieve in the manner described in 2.3 of Part I of this standard. 18.104.22.168 The material coarser than the 1*70-mm IS Sieve shall be washed dried in an oven at 105 to 110Â°C to a substantially constant weight, and accurately weighed to the nearest gram. NOTE -Attention is called to the fact that valuable information concerning the uniformity of the sample under. test may be obtained by determining the lossafter 100 revolutions. When this determination is made, care should be taken to avoid loss of any part of the sample; the entire sample, including the dust of abrasion, shall be returned to the testing machine for the completion of the test.
5.3.5 Reporting of Results-The difference between the ciriginal weight a;d the final weight of the test sample shall be expressed as a percentage of the original weight of the test sample. This value shall be reported as the percentage of wear. 6. DETERMINATION
OF THE POLISHED-STONE
object of this test is to determine the polished-stone 6.1 General -The balue which ,gives a relative measure of the extent to which different types The results of roadstone in the wearing surface will polish under traffic. of this test are used for comparative purposes only; limits cannot, at present, be specified for the polished-stone value in any particular set of circumstances. Where the wearing surface of a road consists largely of stone, the state of polish of the stone will be the dominant factor but other factors also affect the resistance of the surface to skidding. The test is in two parts: a) Samples of stone are subjected special machine.
to an accelerated
polishing action in a
6) The state of polish reached by each sample is measured by means of a suitable friction test and is expressed as the â€˜polished-stone valueâ€™. 6.2 Apparatus
a) An accelerated
shall consist of the following: machine 19
(see Fig. 4) which shall be rigidly1
IS : 2386 (Part IV) - 1963 mounted on a firm, level and non-resilient and shall include:
road wheel having a fiat periphery, and of such a size and shape as to permit fourteen of the specimens to be clamped on the periphery so as to form a continuous surface of stone particles 45 mm wide and 405 mm in diameter.
Means for rotating the road wheel about its own axis at a speed of 320 to 325 rev/min.
3) Means for bringing the surface of a rubber-tyred wheel of 20 cm diameter and 5 cm breadth to bear on the stone surface of the road wheel with a total load of 40 kg. The tyre shall be an industrial 8 x 2 pneumatic 4-ply rating smooth hand-truck tyre with a hardness of 55 &5* and shall be inflated to a pressure of 3.15 fO* 15 kg/cm2. It shall be free to rotate on its own axis, which shall be parallel with the axis of the road wheel; the plane of rotation of the tyre shall be accurately in line with that of the road wheel. Before a new tyre is used on an actual test, it shall be given a preliminary run of 3 hours with sand and 3 hours with emery flour, as in an actual test, but using spare specimens. The tyre shall be discarded after 30 test runs have been made with it, or sooner if it shows signs of irregular wear. 4) Means to feed the sand specified in 6.3 and water at a uniform rate and in such a way that the sand and water are continuously and uniformly spread over the surfaces of the tyre and the specimens where they are in cotitact. This requires about 12 g/min of sand and 20 g/min of water. 5) Means to feed the emery powder specified in 6.3 and water a a uniform rate and in such a way that the emery powder and water are continuously and uniformly spread over the surface of the tyre and the specimens where they are in contact. This fequires about 2 g/min of emery powder and 5 g/min ofwater. b) A friction _ ^_ and 6.7. c) The
with the requirements
set out in 6.6
IS Sieves shall be of the following sizes :
10 mm, 8-O mm (both perforated plate), 425 microns, 212 microns and 150 microns (fine mesh).
*Appendix C of IS : 809-1957 Specification for Rublser Flooring Materials for Genera â€˜Purposes ( Since revised ) gives the method of determining the hardness. 20
IS : 2386 (Part IV) - 1963
SPECIMEN AND APPARATUS FOR ACCELERATED POLISHING
IS : 2386 (Part IV) - 1963 6.3 Materials - A supply of clean, hard siliceous sand, graded within the, following limits ; about 2.5 kg will be required for each test run : Percentage by
Paxsing IS Siece 425-micron 300-micron 2 12-micron 150-micron
100 85-100 20-50 o-5
A supply of air-floated emery powder, 100 percent finer than 0.06 mm and not less than 70 percent finer than 0.002 mm; about 350 g will be required for each test run. 6.4 Preparation of Specimens - At least 3 kg of IO-mm particles shall be available for each sample to be tested. The particles actually used in the preparation of the test specimens shall all pass the IO-mm IS Sieve and be retained on the 8-O-mm IS Sieve and shall be neither flaky nor elongated. These shall be clean and free from dust. 6.4.1 When it is desired to test materials larger than 10 mm which may have characteristics differing from particles of the test size, the particles for the sperimen should be obtained by crushing the larger particles. 6.4.2 Each specimen shall consist ofa single layer of40 to 50 ofthe particles spaced ag closely as possible and covering an area of 90.5 x44.5 mm, set in a sand-cement mortar* with their exposed surfaces proud of the mortar. The surface of the specimen shall be flat across the shorter dimension but shall be curved in the arc of a circle of 400 mm diameter along the longer The individual particles shall be mounted in such a way that dimensfon. the surfaces exposed to wear are as nearly flat as possible, and in any case : resent no sharp edges to the polishing tyre. The specimens shall be not Qess than 12.5 mm thick, and shall be of such a shape as to permit their being clamped round the flat periphery of the road wheel of the accelerated polishing machine so as to form a continuous outer surface of particles with an outer diameter of 405 mm. At least two specimens shall be made from each material to be tested. 6.5 Accelerated Polishing of Specimens -The specimens shall be rigidly clamped round the periphery of the road wheel of the accelerated polishing machine; the wheel will accommodate 14 specimens, and it has been found useful when mounting the specimens on the wheel to insert strips of polythenet about O-25 mm thick between and beneath them. The pneumatic-tyred wheel shall be brought to bear on the surface of the *The mortar shall consist of a mixture of equal portions by weight of the sand specified in 6.3 and high-alumina cement. It is desirable to reinforce each specimen with 3 pieces of 1,2 mm iron wire laid along the longer dime&on. tit should be noted that the name ‘polytbene’ is equivalent to the name ‘polyethylene’.
IS : 2386 (Part IV) - 1963 epecimcns with a total load of 40 kg and the road wheel started up and brought. to a speed of 320 to 325 rev/min. Water and the sand specified in 6.3 shall be fed continuously at the rates specified in 6.2 (a) on the road wheel while it rotates at 320 to 325 rev/min for a period of 3 hours f.5 min. 6.5.1 The machine and specimens shall then be thoroughly cleaned by washing so that all traces of sand are removed and the machine operated for a further three hours as described in 6.5, except that in place of the sand and water the air-floated emery powder specified in 6.3 and water shall be fed continuously at the rates specified in 6.2 (a). After 3 hours &5 min running with the emery powder, the machine shall be stopped and the machine and specimens cleaned. The specimens after polishing are extremely sensitive to handling, and fingering of the polished surfaces shall be avoided. The specimens shall then be tested on the friction tester as described in 6.6. 6.6 Friction Tester-The friction test shall be made with a tester (see Fig. 5) constructed to drawings supplied by the Road Research Laboratory, UK. The tester shall provide: a) a spring-loaded rubber slider of the weight, size and shape specified below, mounted on the end of a pendulum arm so that the sliding edge 1s 50 cm from the axis of suspension. b) means for setting the column of the instrument
c) means for rigidly locating one of the curved specimens from the accelerated polishing machine with its longer dimension in the track of the pendulum, centrally with respect to the rubber slider and to the axis of suspension of the pendulum. d) means for raising and lowering the axis of suspension of the pendu!um so that the slider can (1) swing clear of the surface of the specimen or (2) be set to slide over a fixed length of surface of 75 f 1.5 mm. e) means for holding and releasing freely from a horizontal position.
arm so that it falls
f) a pointer balanced about the axis of suspension indicating the position of the pendulum arm throughout its forward swing, and moving over a circular scale drawn up as specified in 6.6.1 to 6.6.3. The weight of the pointer shall be not more than 85 g and the friction in the pointer mechanism shall be adjustable so that, with the pendulum arm swinging freely from a horizontal position, the outward tip of a 30-cm long pointer may be brought to rest on the forward swing of the arm at a point 10 mm below the horizontal. 6.6.1 The weight of the swinging arm including the slider shall be 1*500& O-025 kg, the centre of gravity lying on the axis of the arm at a distance of 905f5 mm from the centre of suspension. 23
IS -: !B86 (Part IV) - 1963
MEASCRE THE COEFFKXNT
OF THE SPECIMEN
6.6.2 The slider shall consist of a rubber pad 32 mm wide and 6.5 mm thick held on a rigid base with a total weight of 25-&Z g which is mounted on an axis set at an angle of20 degrees with the horizontal when the pendulum is at the lowest point of its swing, so that (a) only the rear edge of the slider contacts the test surface, and (b) the slider can turn about its axis without obstruction to follow unevenness of the surface, perpendicular to the plane of the pendulum swing. The slider shall be spring loaded against the test surface and the load on the slider shall be 2.2510.05 kg in its mean position; the change in load on the slider shall be not greater than 190 g/cm deflection of the slider. 6.6.3 The slidrr shall be made from rubber tested and specially selected rfor the purpose. Before use, each working end of a new slider shall be 24
IS : 2386 (Part IV) - 1963 roughened by swinging it at least 10 times over which shall not be one of the specimens to be used for not more than 500 swings with each shall, in any case, be discarded not more than supplied.
a dry, unpolished specimen, tested. Each slider shall be of the two usable ends, and one year after the date it is
NOTE Recent rcsra~~h has thrown new light on the properties of rubber that govern i!s frictionai rrsistance. Until the results of this research can be applied on a commercial scale, it is essential that the rubber for we in the slider be carefully tested and selected. When so selected, it should last without any ageing effect for at least a year; full instructions on this and other points relating to the use of the portable tester are issued with eacK instrument.
6.6.4 All bearings and working parts of the instruments shall be enclosed as far as possible, and all materials used shall be suitably treated to prevent corrosion under wet conditions. 6.7 Calibration of the Tester -- The scale of the instrument when used for this test shall give the coefficient of friction, expressed as a percentage, and shall be drawn up by means of the following equation:
wxz x PDP
7 effective coefficient
expressed as a percentage;
weight in kg of the swinging arm;
X = distance in cm of the effective the centre of oscillation;
centre of gravity of the arm from
< = vertical distance of the edge of the scale below the zero of the scale, ,which shall he 10 mm below the horizontal when the arm is released to swing freely from the horizontal ;
P = normal load in kg on the slider; D = sliding distance
in cm; and
P = length in cm of the pointer. The instrument shall be cross-checked with the Road Research standard machine.on the following wetted surfaces:
a) A glass plate. b) Five smooth-looking surfaces having a texture depth less than 0.25 mm and covering a range of coefficients of friction, , expressed as a percentage, of atâ€˜ieast 25-to 75 percent. c) Five rough-looking surfaces having a texture depth greater than 0.51 mm and covering a range of Ooefficients of friction, expressed as a percentage, of at least 35 to 70 percent. 25
IS : 2386 (Part IV) - 1963 On these tests no pairs of results on any surface shall differ by more than f3 percent and the mean results for the 11 samples shall not differ by more than h1.5 percent. 6.6 Friction of 20 f2”C.
The test shall be made at a temperature
6.8.1 The tester shall rest upon a firm level surface and the levelling screws shall be adjusted so that the column is vertical. The axis of suspension of the pendulum shall then be raised so that the arm swings freely, and the friction in the pointer mechanism shall be adjusted so that when the pendulum arm and pointer are released from the right-hand horizontal position the pointer comes to rest at the zero position on the scale. 6.8.2 The specimen shall then be rigidly located with its longer dimension lying in the track of the pendulum, and centrally with respect to the rubber slider and to the axis of suspension of the pendulum. The height of the axis of suspension of the pendulum shall then be adjusted so that in traversing the specimen the rubber slider is in contact with it over the whole width of the slider and over a length of 75 & 1*5’mm of the specimen under a normal load of 2*25&O-05 kg. The surfaces of the specimen and the rubber slider shall then be wetted with a copious supply of clean water, care being taken not to disturb the slider from its set position. The pendulum and pointer shall then be released from the horizontal position and the reading of the pointer recorded to the nearest whole number. 6.8.3 The procedure same material.
shall then be repeated with a second specimen
6.8.4 If the values obtained 3 percent, a further specimen agree within this limit.
from the two specimens differ by more than or specimens shall be tested until two values
NOTE-If the tester has not been used for eight hours previously, five swings shall be made on a spare specimen before an actual test is made.
6.9 Reporting of Results - The mean of the two values of the coefficient of friction, expressed as a percentage, shall be reported to the nearest whole number as ‘follows : Laboratory
7.1 General - When aggregates are not available, this test may be used to give a direct measure of the stress in kg/cm2 at ultimate failure of a rock under a slowly increasing compressive load.
-_-*This is not, and should not be confused with, the ‘Sideway force coeBicient’ or the ‘Skidresistance value’ determined on a road.
IS: 7.2 Apparatus
shall consist of the following:
a) A compression testing machine of suitable capacity and at least one platen having a spherical seating of not more than 2.5 cm radius. b) A well-ventilated oven, thermostatically temperature of 100 to 110Â°C.
7.3 Test Specimens - The test specimens shall be cylinders of 25*0*5 mm mean diameter and of 25 f0.5 mm mean height. In any one specimen, the diameter shall not vary by more than 0.25 mm and the height by not The end faces shall be at right angles to the cylindrical more than 0.15 mm. axis and shall be lapped plane to an accuracy of O-025 mm. 7.3.1 The samples from which the test specimens are prepared shall be taken from freshly quarried material and only from pieces which show no When planes of structural weakness are evidence of incipient fracture. discernible, the sample shall be so selected as to furnish some test specimens with the planes of structural weakness at right angles to the cylindrical axis of the specimen. 7.3.2 The size of the samples shall be approximately 8 x4 x4 cm if the test specimens are to be prepared by grinding only and 15 x 15 x 10 cm of the test specimens are to be prepared by drilling, sawing and grinding. 7.3.3 In the preparation of the test specimens, the rock shall not be subjecTtd to any treatment (such as chipping with a hammer) liable to induce A copious flow of cold water shall be used throughout incipient fracture. all grinding, drilling and sawing operations, to ensure that the aggregate is not damaged by overheating. 7.3.4 The test specimens shall be dried for four hours in the oven at a temperature of 100 to 110Â°C and cooled before test. 7.3.5 If no planes of structural weakness are apparent, three specimens shall be tested. If planes of structural weakness are apparent, four specimens shall be tested, of which two shall have the planes at right angles to the axis of the cylinder. 7.4 Procedure-The diameter and height of each specimen shall be measured to an accuracy of 0.025 mm. The specimen shall be placed centrally between the steel platens without packing. 7.4.1 Each test shall be a direct compression test in which the load is applied to the ends of the cylindrical test specimen at a rate of about 5 In making each test, the final load necessary to produce tonnes per minute. crushing of the specimen shall be observed. 75 Calculations - The stress shall be calculated sectional area of the specimen.
in kg/cm* from the cross-
IS : 2386 (Part IV) - 1963 7.6 Reporting of Results - The value of the crushing stress for each individual specimen, and the average crushing stress shall be reported to the nearest 5 kg/cm2. Any peculiar condition ofa test specimen which might affect the result of the test, such as the presence of seams, fissures, etc, shall be noted in the report.
Headquarters: Manak Bhavan, 9 Bahadur Shah Zafar Marg, NEW DELHI 110002 Telephones: 323 0131, 323 3375, 323 9402 Fax :91113234062, 91113239399, 91113239382 Telegrams : Manaksanstha (Common to all Offices) Telephone
Central Laboratory: Plot No, 20/9, Site IV, Sahibabad
8-77 00 32
: Manak Bhavan, 9 Bahadur Shah Zafar Marg, NEW DELHI 110002 : l/l4 CIT Scheme VII M. V.I.P. Road, Maniktola, CALCUTTA700054
Central ‘Eastern Northern
335-336, Sector 34-A, CHANDIGARH
60 38 43
: C.I.T. Campus, IV Cross Road, CHENNAI 600113 tWestern : Manakalava. E9 Behind Mar01 Telephone Exchange, Andheri (East),
323 76 17 337 86 62 235 23 15 832 92 95
Branch Offices: ‘Pushpak’,
Shaikh Marg. Khanpur. AHMEDABAD
5th Floor, Bhadbhada
Road, T. T. Nagar, BHOPAL 462003
Plot No. 62-63, IJnit VI. Ganga Nagar, BHUBANESHWAR Kalaikathir
Buildings, 670 Avinashi Road, COIMBATORE
Plot No. 43, Sector 16 A, Mathura Savitri Complex,
116 G. T. Road, GHAZIABAD
L. N. Gupta Marg, Nampally
21 01 41
8-28 88 01
8-71 19 96
1171418 B, Sarvodaya
Station Road, HYDERABAD
55 40 21 40 36 27
53/5 Ward No. 29, R. G. Barua Road, 5th By-lane, GUWAHATI 781003 5-8-58C,
550 13 48 839 49 55
SPeenya Industrial Area, 1st Stage, Bangalore - Tumkur Road, BANGALORE 560058
54 11 37 20 10 83 37 29 25
21 68 76
Seth Bhawan, 2nd Floor. Behind Leela Cinema, Naval Kishore Road, LUCKNOW 226001
23 89 23
26 23 05
Estate, PATNA 800013
T. C. No. 1411421, University THIRUVANANTHAPURAM
6 21 17
P. 0. Palayam. 695034
NIT Building, Second Floor, Gokulpat Market, NAGPUR Institution
( India ) Building, 1332 Shivaji Nagar, PUNE 411005
52 51 71 32 36 35
I ‘Sales Office is at 5 Chowringhee CALCUlTA 700072 tSales
Office is at Novelty Chambers,
F’. 0. Princep Street, 271085
Grant Road, MUMBAI
*Sales Office is at ‘F’ Block, Unity Building, Narashimaraja BANGALORE 560002
309 65 28 222 39 71
Printed at New India Prlntlng Press, Khurja. India
AMENDMENT NO. 2
TO IS:2386(Part IV)-1963 METHODS OF TEST FOR AGGREGATES FOR CONCRETE PART IV
MECHANICAL PROPERTIES Alterations ------
(Page 8, Note I under thee Delete.
2.6, Zast sentence) -
(Page 13, clause 5.1) - Substitute the following for the existing clause: '5.1 OJQe& - This test covers the method of determining the abrasion value of coarse w,rrgate by the use of Los Angeles machine (see 5.2),' (Pages 14 to 16, clause8 5.2 to 5.2.7) - Delete and renumber the subsequent clawes accordingly.
Printed at New India Printing Press, Khuja, India
IS : 2386 ( Part IV ) - 1963 TEST FOR AGGREGATES PART
METHODS OF FOR CONCRETE
Alterations ( Page 5,
2.2 ) -
for the existing
clause: ‘ 2.2 Apparatus the following:
for the standard
a) An open-ended 150 mm cylindrical cell with appropriate base plate and plunger, metal measure and tamping rod conforming to IS : 9376-1979 Specification for apparatus for measuring aggregate crushing value and ten percent fines value; b) A balance
3 kg readable
c) IS sieve of sizes 12.5 mm,
to one gram;
10 mm and 2.36 mm; and
d) A compression testing machine capable of applying a load of 40 tonnes in not more than 10 minutes at a uniform rate 01’ loading. The machine may be used with or without a spherical seating. ( Page existing:
1, .Note ) -
6.5 kg of natural aggregates is required to provide two test ‘ NOTE-About samples for 15 cm cylinder and about 1 kg for 7.5 cm cylinder. For lightweight aggregates, the quantity will vary depending on the density of the aggregate.’ ( Page 6, Fig.
2.3.2 ) -
for the existing
clause: 6 2.3.2 The quantity of aggregate shall be such that the depth material in the cylinder, after tamping as described in 2.3.3, shall about 10 cm.’ ( Page 8, clause 2.6 Note 1, last sentence ) 1
clause 2.6 Note 2 ) -
the following No,te for the
‘NOTE 2 - Agqregales smallrr than 10 mm - In general the smaller sizes of aggrebetween the gates will give a lower aggregate crushing value, but the relationsbip values obtained with different sizes will vary from one aggregates to another. The tests on smaller aggregates may be made either using the standard apparatus described in 2.2 or a smaller apparatus consisting of a 75 mm cylindrical cell with aprpopriate accessories conforming to IS : 9376-1979 Specification for apparatus for measuring aggregates crushing value and ten percent fines value. In case a smaller apparatus is used, the errors for the smaller sizes of aggregate tested in the smaller apparatus are compensated since the results obtained with the smaller apparatus have been found to be slightly higher than those with the standard apparatus,
500 g, Table in not smaller 50 mm (
The accessories for the smaller apparatus shall be a balance of readable and accurate to @2 g; IS sieves of appropriate sizes as 1; and a compression testing machine capable of,applying a load of more than 10 min at a uniform rate of loading. Further, in the test apparatus, the depth of material in the 75 mm cylinder shall and the total load applied in 10 min shall be 10 tonnes.’
Pages 8 and 9, clause 3.2 ) -
( 3.2 Apparatus -
capacity given in 10 tonnes using the be about
Substitute the following for the existing
The apparatus shall consist of the following:
a) A 150 mm cylindrical cell with appropriate plunger and base plate, tamping rod and metal measure conforming to IS : 93761979 Specification for apparatus for measuring aggregate crushing value and ten percent fines value; b) A balance of capacity 3 kg, readable and accurate to one gram; c) IS sieves of sizes 12.5 mm, 10 mm and 2.36 mm; d) A compression testing machine capable of applying a load of 50 tonnes in not more than 10 minutes at a uniform rate of loading. The load may vary from O-5 to 50 tonnes; and e) A means of measuring the reduction in the distance between the platens of the testing machine to the nearest one mm during the test ( for example, a dial gauge). ( Page 9, clause 3.3.2 ) -Substitute clause:
for the existing
‘ 3.3.2 The quantity of aggregate shah be such that the depth of material in the cylinder, after tamping as described in 22.214.171.124, shall be about 10 cm.’ [ Page 19, clause 126.96.36.199 ( see also Amendment No. 2 ), fhird line ] Substitute ‘ 30 to 33 rev/min ’ for ( 20 to 33 rev/mm ‘. [ Page 19, clause 5.3.5 ( see also Amendment No. 2 ) ] the following for the existing clause:
‘ 5.3.5 Reporting of Results - The difference between the original weight and the final weight of the test sample shall be expressed as a percentage 2
of the original weight of the test Qample. be reported as the percentage of wear. ’
The mean of two results shall
( Pagts 26, 27 and 28, clauses 7 to 7.6 ) -
Addendom ( Pap
2.3.3 ) -Add
the following at the end of the clause:
‘( see Note given in Table 1 )’
Published on Mar 10, 2018